# Computational Crystal Plasticity : From Single Crystal to ... Computational Crystal Plasticity :...

date post

14-Aug-2020Category

## Documents

view

3download

0

Embed Size (px)

### Transcript of Computational Crystal Plasticity : From Single Crystal to ... Computational Crystal Plasticity :...

TECHNISCHE MECHANIK,Band 23, Heft 2-4, (2003), 130– 145 Manuskripteingang: 1. Juli 2003

Computational Crystal Plasticity : From Single Crystal to Homogenized Polycrystals

G. Cailletaud, O. Diard, F. Feyel, S. Forest

Jürgen Olschewski zum Gedächtnis

Crystal plasticity models for single crystals at large deformation are shown. An extension to the computation of polycrystals is also proposed. The scale transition rule isnumerically identified on polycrystal computations, and is valid for any type of loading. All these models are implemented in a finite element code, which has a sequential and a parallel version. Parallel processing makes CPU time reasonable, even for 3D meshes involving a large number of internal variables (more than 1000) at each Gauss point.

Together with a presentation of the numerical tools, the paper shows several applications, a study of the crack tip strain fields in single crystals, of zinc coating on a steel substrate, specimen computation involving a large number of grains in each Gauss point. Finally, polycrystalline aggregates are generated, and numerically tested. The effect of grain boundary damage, opening and sliding is investigated.

1 Introduction

Continuum crystal plasticity encompasses a large class of now wide–spread models accounting for the anisotropic deformation of metal single crystals. Its roots are to be found in the works of Taylor, but the complete finite deformation framework is due to the successive contributions of Bilby, Kröner, Teodosiu, Rice and finally Man- del (1973). It is the appropriate framework to simulate the deformation of single crystal specimens under complex loading conditions (tension, shear, torsion, channel die,etc.), but also single crystal components like turbine blades in jet engines (Forest et al. (1996)). Crystal plasticity can be used also to derive the behavior of metal polycrys- tals from the behavior of individual grains. Such models arenow available at two levels. The most predictive version consists in considering sets of interacting grainswith a sufficient description of the transgranular behavior (Mika and Dawson (1998); Staroselsky and Anand (1998); Barbe et al. (2001b); Böhlke and Bertram (2001)). This delivers three classes of information : the overall response of the considered material volume that may be close to the wanted effective behavior of the polycrystal, the mean stress and strain for grains having similar crys- tal orientations, and, finally, the complete heterogeneousstress/strain distribution inside individual grains. The results are obtained through considerable computational effort. That is why simplified homogenization models accounting only for the two first previous information levels are useful. The estimations provided by the Taylor or self–consistent schemes can capture the initial and strain–induced anisotropy of polycrystal behavior from the knowledge of single crystal behavior and material texture described by the orientation distribution function (see references quoted in Cailletaud et al. (2003)). Such modelsare now very efficient regarding computation time and quality of prediction, so that they can be used for industrial purposes like prediction of texture evolution in metal forming. They can even be included in finite element simulations (Beaudoin et al. (1993); Cailletaud and Pilvin (1994)).

The aim of the present work is to illustrate the panel of computational crystal plasticity models that are now available to describe accurately material behavior ranging from single crystal specimens to polycrystalline metals and alloys. The gain in using such an approach instead of traditional purely phenomenological constitutive theories is emphasized. The computational cost of the use of such methods will be shown to be now attractive enough to compete with more standard design methods. This has to be related to the development of new computational techniques, involving parallel computations, which are specially competitive for this class of models. A short presentation of the used methods will be given. One also includes new advances that push forward the limitations of the classical approach : accounting for size effects, damage and specific grain boundary behavior, etc.

130

The present work is divided into four main parts. In the first one, the continuum crystal plasticity framework is introduced, starting from a representation of dislocation distribution inside the single crystal volume element. Finite element (FE) computations of stress/strain fields atthe crack tip in single crystals are shown as an example. The second one deals with the computation of multicrystalline aggregates. Multicrystals are said here to contain a rather small number of grains, so that the specimen or the component they belong to can be completely meshed with the real grain orientations. The approach is applied tomulticrystalline metal coating. The topic of the next part is a discussion of the various scales in an aggregate; a simplified uniform field model involving an explicit scale transition rule is presented. An application in an FE code isshown. The last part concentrates on polycrystalline aggregates, i.e. computational models of a representativevolume element (RVE), often artificially generated, to represent bulk polycrystalline metals. Local responses ona granular and intragranular level are analyzed. They demonstrate that grain boundaries play a critical role in the polycrystal behavior. This is the reason why a last type of modeling, including an explicit mesh of the grain boundaries is finally proposed.

2 Single Crystal Plasticity

2.1 Generalized vs. Classical Crystal Plasticity

Continuum crystal plasticity theory aims at establishing acontinuum mechanical framework accounting for the result of complex dislocation glide, multiplication and interaction processes at work in plastically deformed met- als. Kröner (1969) proposed to retain the following statistical information out of the intricate entanglement of dislocations contained in a single crystal material volumeelement :

• the dislocation density tensorα ∼

represents the ensemble average of the tensor product of thedislocation line and Burgers vectors. It is the basic variable of the continuum theory of disclocations and can be directly related to the densities of so–calledgeometrically necessary dislocationsρG introduced by Ashby (1971).

• the scalar dislocation densityρS denotes the total length of dislocation lines contained in agiven volume. It is the basic measure in physical metallurgy and is responsible for a large part of material hardening.

The classical crystal plasticity framework settled by Mandel (1973) and further developed and summarized by Asaro (1983) and Cuitiño and Ortiz (1993), take only the second dislocation density measure into account. It has proved to be a well–suited tool to describe homogeneous and slightly heterogeneous deformation and hardening of single crystals under complex loading conditions. It is based on the definition of crystallographic directors and the introduction of a unique so–called isoclinic intermediateconfiguration for which the orientation of the directors coincides with the initial one :

F ∼

= E ∼ .P ∼ , Ṗ

∼ .P ∼ −1 =

N

∑ s=1

γ̇sms⊗ns (1)

where the deformation gradient isF ∼

, the elastic and plastic deformation tensors areE ∼

andP ∼

respectively. The amount of plastic slip on each slip systems is denoted byγs. The vectorsms andns represent the slip direction and normal to the slip plane respectively. In the present work, aviscoplastic framework is adopted, together with the classical Schmid law to trigger plastic glide :

γ̇scum= 〈

|τs−xs|− rs

k

〉n

, γ̇s = γ̇scumsign(τ s−xs) (2)

whereτs, rs andxs denote the resolved shear stress, the isotropic and kinematic hardening variables, respectively. The isotropic hardening variable is the thermodynamical force associated with an internal variable which usually is more or less directly related to the dislocation densities ρs. Identifications and applications of such constitutive equations can be found in Méric et al. (1991); Forest et al. (1996) and Cailletaud et al. (2003).

As acknowledged by Mandel (1973) and Sidoroff (1975), the previous classical formulation is a simplified version of a more general model that should incorporate at least the two dislocation density measures introduced at the beginning of this Section. Indeed, such generalized formulations of crystal plasticity have been proposed for instance by Fleck and Hutchinson (1997) and Forest et al. (1997). According to the latter framework, the rotation of the crystal directors is regarded as an actual degree of freedom of the material point independent from its displacement. This leads to the identification of the dislocated crystal with a Cosserat continuum. The kinematics of Cosserat crystal plasticity is illustrated by Fig. 1. Thegradient of the lattice rotation tensor is called the lattice

131

F

E P

Γ

ΓΓ p e

~

~~ ~

~

~

Figure 1: Kinematics of Cosserat single crystal plasticity.

torsion–curvature tensorΓ ∼ , the plastic part of which directly influences the hardeningof the material. This can be

seen in the following generalized non–linear isotropic hardening rule

rs = r0 +Q N

∑ r=1

hsr(1−exp(−bγrcum))+Hlcκ s (3)

The two first terms are the initial critical resolved shear stress and subsequent non–linear hardening including the interaction matrixhrs between the slip syst

*View more*